#------------------------------------------------------------------------------
#$Date: 2016-03-21 18:51:55 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178827 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/81/4108193.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4108193
loop_
_publ_author_name
'Guanggang Gao'
'Fengyan Li'
'Lin Xu'
'Xizheng Liu'
'Yanyan Yang'
_publ_section_title
;
 CO2 Coordination by Inorganic Polyoxoanion in Water
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              10838
_journal_page_last               10839
_journal_paper_doi               10.1021/ja801560t
_journal_volume                  130
_journal_year                    2008
_chemical_formula_moiety
;
C Co Mo11 O40 Si, 4(C3 H5 N2), 4(H2 O) 
;
_chemical_formula_sum            'C13 H28 Co Mo11 N8 O44 Si'
_chemical_formula_weight         2142.75
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           69
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-F 2 2'
_symmetry_space_group_name_H-M   'F m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.039(1)
_cell_length_b                   21.333(2)
_cell_length_c                   21.889(2)
_cell_measurement_reflns_used    3865
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.48
_cell_measurement_theta_min      1.80
_cell_volume                     6088.7(9)
_computing_cell_refinement       'SMART (Bruker, 2002)'
_computing_data_collection       'SMART (Bruker, 2002)'
_computing_data_reduction        'SAINT (Bruker, 2002)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  SHELXTL
_computing_structure_solution    'SHELXTL (Bruker, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.976
_diffrn_measured_fraction_theta_max 0.976
_diffrn_measurement_device_type  'Smart CCD Apex II'
_diffrn_measurement_method       'omega and phi'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0264
_diffrn_reflns_av_sigmaI/netI    0.0159
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            12685
_diffrn_reflns_theta_full        26.01
_diffrn_reflns_theta_max         26.01
_diffrn_reflns_theta_min         2.05
_exptl_absorpt_coefficient_mu    2.567
_exptl_absorpt_correction_T_max  0.685
_exptl_absorpt_correction_T_min  0.620
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2002)'
_exptl_crystal_colour            'dark brown'
_exptl_crystal_density_diffrn    2.329
_exptl_crystal_description       block
_exptl_crystal_F_000             4036
_exptl_crystal_size_max          0.224
_exptl_crystal_size_mid          0.163
_exptl_crystal_size_min          0.152
_refine_diff_density_max         0.844
_refine_diff_density_min         -0.849
_refine_diff_density_rms         0.140
_refine_ls_extinction_coef       0.00036(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     122
_refine_ls_number_reflns         1623
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.046
_refine_ls_R_factor_all          0.0621
_refine_ls_R_factor_gt           0.0561
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0841P)²+154.2864P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1118
_refine_ls_wR_factor_ref         0.1383
_reflns_number_gt                1434
_reflns_number_total             1623
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja801560t-file.003.cif
_cod_data_source_block           si
_cod_database_code               4108193
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-x, -y+1/2, -z+1/2'
'x, y+1/2, -z+1/2'
'x, -y+1/2, z+1/2'
'-x, y+1/2, z+1/2'
'-x+1/2, -y, -z+1/2'
'x+1/2, y, -z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y, z+1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Si Si 0.5000 0.5000 0.0000 0.0308(9) Uani 1 8 d S
Mo1 Mo 0.23566(10) 0.5000 0.0000 0.0501(5) Uani 0.64 4 d SP
Mo2 Mo 0.36289(6) 0.38314(3) 0.08076(4) 0.0555(4) Uani 1 1 d .
Mo3 Mo 0.5000 0.5000 0.15964(6) 0.0489(4) Uani 0.86 4 d SP
Co1 Co 0.23566(10) 0.5000 0.0000 0.0501(5) Uani 0.36 4 d SP
Co2 Co 0.5000 0.5000 0.15964(6) 0.0489(4) Uani 0.14 4 d SP
O1 O 0.5000 0.4577(5) 0.0605(6) 0.036(3) Uani 0.531(19) 2 d SP
O1' O 0.3979(8) 0.4536(5) 0.0000 0.028(3) Uani 0.469(19) 2 d SP
O2 O 0.0994(10) 0.5000 0.0000 0.074(4) Uani 1 4 d S
C1 C 0.0000 0.5000 0.0069(5) 0.11(3) Uani 0.5 4 d SP
O3 O 0.2572(8) 0.4370(4) 0.0623(3) 0.099(2) Uani 1 1 d .
O4 O 0.3573(11) 0.3489(6) 0.0000 0.105(4) Uani 1 2 d S
O5 O 0.3020(6) 0.3263(3) 0.1180(4) 0.085(2) Uani 1 1 d .
O6 O 0.5000 0.3501(5) 0.0841(7) 0.099(4) Uani 1 2 d S
O7 O 0.3978(5) 0.4383(4) 0.1449(5) 0.096(3) Uani 1 1 d .
O8 O 0.5000 0.5000 0.2361(7) 0.095(5) Uani 1 4 d S
OW1 O 0.187(2) 0.5000 0.1767(12) 0.100(7) Uiso 0.50 2 d SP
OW2 O 0.2500 0.3971(13) 0.2500 0.104(7) Uiso 0.50 2 d SP
N1 N 0.4138(19) 0.2060(15) 0.0000 0.146(11) Uiso 1 2 d SPD
H1 H 0.3513 0.2188 0.0000 0.175 Uiso 1 2 calc SR
N2 N 0.419(3) 0.1986(18) 0.1844(15) 0.148(10) Uiso 0.50 1 d P
H2A H 0.3560 0.2081 0.1772 0.177 Uiso 0.50 1 calc PR
C2 C 0.5000 0.2398(9) 0.0000 0.083(7) Uani 1 4 d SD
H2 H 0.5000 0.2834 0.0000 0.100 Uiso 1 4 calc SR
C3 C 0.4491(16) 0.147(2) 0.0000 0.22(3) Uiso 1 2 d SPD
H3 H 0.4082 0.1108 0.0000 0.259 Uiso 1 2 calc SR
C4 C 0.5000 0.2335(14) 0.1665(15) 0.082(9) Uani 0.50 2 d SP
H4 H 0.5000 0.2721 0.1468 0.098 Uiso 0.50 2 calc SPR
C5 C 0.444(3) 0.1551(15) 0.2102(18) 0.162(17) Uani 0.50 1 d P
H5 H 0.4020 0.1252 0.2280 0.194 Uiso 0.50 1 calc PR
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Mo1 O3 98.3(3) . 19_565
O2 Mo1 O3 98.3(3) . 18
O3 Mo1 O3 163.3(6) 19_565 18
O2 Mo1 O3 98.3(3) . 4_565
O3 Mo1 O3 89.6(5) 19_565 4_565
O3 Mo1 O3 88.0(5) 18 4_565
O2 Mo1 O3 98.3(3) . .
O3 Mo1 O3 88.0(5) 19_565 .
O3 Mo1 O3 89.6(5) 18 .
O3 Mo1 O3 163.3(6) 4_565 .
O2 Mo1 O1' 154.9(3) . 19_565
O3 Mo1 O1' 64.8(3) 19_565 19_565
O3 Mo1 O1' 99.4(4) 18 19_565
O3 Mo1 O1' 64.8(3) 4_565 19_565
O3 Mo1 O1' 99.4(4) . 19_565
O2 Mo1 O1' 154.9(3) . .
O3 Mo1 O1' 99.4(4) 19_565 .
O3 Mo1 O1' 64.8(3) 18 .
O3 Mo1 O1' 99.4(4) 4_565 .
O3 Mo1 O1' 64.8(3) . .
O5 Mo2 O3 101.9(4) . .
O5 Mo2 O7 101.8(4) . .
O3 Mo2 O7 87.4(3) . .
O5 Mo2 O4 99.0(6) . .
O3 Mo2 O4 90.4(4) . .
O7 Mo2 O4 159.1(5) . .
O5 Mo2 O6 99.1(5) . .
O3 Mo2 O6 159.1(5) . .
O7 Mo2 O6 88.6(4) . .
O4 Mo2 O6 86.0(5) . .
O5 Mo2 O1' 157.2(4) . .
O3 Mo2 O1' 65.4(4) . .
O7 Mo2 O1' 96.5(4) . .
O4 Mo2 O1' 63.9(5) . .
O6 Mo2 O1' 94.7(5) . .
O5 Mo2 O1 156.4(4) . .
O3 Mo2 O1 95.9(4) . .
O7 Mo2 O1 63.3(4) . .
O4 Mo2 O1 96.3(6) . .
O6 Mo2 O1 64.1(4) . .
O1' Mo2 O1 46.1(4) . .
O8 Mo3 O7 99.8(3) . .
O8 Mo3 O7 99.8(3) . 2_665
O7 Mo3 O7 160.5(6) . 2_665
O8 Mo3 O7 99.8(3) . 20_655
O7 Mo3 O7 89.0(4) . 20_655
O7 Mo3 O7 87.7(5) 2_665 20_655
O8 Mo3 O7 99.8(3) . 19_565
O7 Mo3 O7 87.7(5) . 19_565
O7 Mo3 O7 89.0(4) 2_665 19_565
O7 Mo3 O7 160.5(6) 20_655 19_565
O8 Mo3 O1 157.4(3) . .
O7 Mo3 O1 65.0(3) . .
O7 Mo3 O1 96.3(4) 2_665 .
O7 Mo3 O1 65.0(3) 20_655 .
O7 Mo3 O1 96.3(4) 19_565 .
O8 Mo3 O1 157.4(3) . 2_665
O7 Mo3 O1 96.3(4) . 2_665
O7 Mo3 O1 65.0(3) 2_665 2_665
O7 Mo3 O1 96.3(4) 20_655 2_665
O7 Mo3 O1 65.0(3) 19_565 2_665
O1 Mo3 O1 45.2(6) . 2_665
Si O1 O1 55.7(4) . 2_665
Si O1 Mo3 123.1(6) . .
O1 O1 Mo3 67.4(3) 2_665 .
Si O1 Mo2 121.2(4) . .
O1 O1 Mo2 130.8(2) 2_665 .
Mo3 O1 Mo2 94.8(4) . .
Si O1 Mo2 121.2(4) . 20_655
O1 O1 Mo2 130.8(2) 2_665 20_655
Mo3 O1 Mo2 94.8(4) . 20_655
Mo2 O1 Mo2 94.6(4) . 20_655
Si O1' Mo1 118.3(6) . .
Si O1' Mo2 122.3(3) . 18
Mo1 O1' Mo2 95.4(3) . 18
Si O1' Mo2 122.3(3) . .
Mo1 O1' Mo2 95.4(3) . .
Mo2 O1' Mo2 96.8(4) 18 .
C1 O2 Mo1 173.4(5) 4_565 .
C1 C1 O2 83.4(5) 4_565 .
O2 C1 O2 166.8(10) 17_565 .
Mo2 O3 Mo1 134.2(5) . .
Mo2 O4 Mo2 134.9(8) 18 .
Mo2 O6 Mo2 136.8(7) 20_655 .
Mo2 O7 Mo3 136.6(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Si O1 1.604(12) 18
Si O1 1.604(12) .
Si O1' 1.659(12) 19_565
Si O1' 1.659(12) 3_655
Mo1 O2 1.777(13) .
Mo1 O3 1.934(8) 19_565
Mo1 O3 1.934(8) 18
Mo1 O3 1.934(8) 4_565
Mo1 O3 1.934(8) .
Mo1 O1' 2.336(11) 19_565
Mo1 O1' 2.336(11) .
Mo2 O5 1.663(6) .
Mo2 O3 1.840(8) .
Mo2 O7 1.887(8) .
Mo2 O4 1.914(5) .
Mo2 O6 1.923(4) .
Mo2 O1' 2.365(8) .
Mo2 O1 2.433(8) .
Mo3 O8 1.673(16) .
Mo3 O7 1.901(7) .
Mo3 O7 1.901(7) 2_665
Mo3 O7 1.901(7) 20_655
Mo3 O7 1.901(7) 19_565
Mo3 O1 2.350(13) .
Mo3 O1 2.350(13) 2_665
O2 C1 1.304(13) 4_565
O2 C1 1.304(13) .
C1 O2 1.304(13) 17_565
N1 C2 1.34(3) .
N1 C3 1.34(5) .
N2 C5 1.14(4) .
N2 C4 1.35(4) .
C2 N1 1.34(3) 3_655
C3 C3 1.33(4) 3_655
C4 N2 1.35(4) 20_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O7 Mo3 O1 Si 129.3(3) . .
O7 Mo3 O1 Si -44.8(2) 2_665 .
O7 Mo3 O1 Si -129.3(3) 20_655 .
O7 Mo3 O1 Si 44.8(2) 19_565 .
O1 Mo3 O1 Si 0.0 2_665 .
O8 Mo3 O1 O1 180.000(3) . 2_665
O7 Mo3 O1 O1 129.3(3) . 2_665
O7 Mo3 O1 O1 -44.8(2) 2_665 2_665
O7 Mo3 O1 O1 -129.3(3) 20_655 2_665
O7 Mo3 O1 O1 44.8(2) 19_565 2_665
O8 Mo3 O1 Mo2 47.5(2) . .
O7 Mo3 O1 Mo2 -3.2(3) . .
O7 Mo3 O1 Mo2 -177.3(3) 2_665 .
O7 Mo3 O1 Mo2 98.2(4) 20_655 .
O7 Mo3 O1 Mo2 -87.6(3) 19_565 .
O1 Mo3 O1 Mo2 -132.5(2) 2_665 .
O8 Mo3 O1 Mo2 -47.5(2) . 20_655
O7 Mo3 O1 Mo2 -98.2(4) . 20_655
O7 Mo3 O1 Mo2 87.6(3) 2_665 20_655
O7 Mo3 O1 Mo2 3.2(3) 20_655 20_655
O7 Mo3 O1 Mo2 177.3(3) 19_565 20_655
O1 Mo3 O1 Mo2 132.5(2) 2_665 20_655
O5 Mo2 O1 Si 174.8(7) . .
O3 Mo2 O1 Si -46.4(6) . .
O7 Mo2 O1 Si -130.5(7) . .
O4 Mo2 O1 Si 44.6(6) . .
O6 Mo2 O1 Si 127.1(8) . .
O1' Mo2 O1 Si 0.7(5) . .
O5 Mo2 O1 O1 -115.5(8) . 2_665
O3 Mo2 O1 O1 23.3(4) . 2_665
O7 Mo2 O1 O1 -60.8(4) . 2_665
O4 Mo2 O1 O1 114.3(4) . 2_665
O6 Mo2 O1 O1 -163.2(6) . 2_665
O1' Mo2 O1 O1 70.5(4) . 2_665
O5 Mo2 O1 Mo3 -51.4(9) . .
O3 Mo2 O1 Mo3 87.4(3) . .
O7 Mo2 O1 Mo3 3.2(3) . .
O4 Mo2 O1 Mo3 178.4(3) . .
O6 Mo2 O1 Mo3 -99.1(5) . .
O1' Mo2 O1 Mo3 134.5(5) . .
O5 Mo2 O1 Mo2 43.7(11) . 20_655
O3 Mo2 O1 Mo2 -177.4(4) . 20_655
O7 Mo2 O1 Mo2 98.4(5) . 20_655
O4 Mo2 O1 Mo2 -86.4(5) . 20_655
O6 Mo2 O1 Mo2 -3.9(5) . 20_655
O2 Mo1 O1' Si 180.0 . .
O3 Mo1 O1' Si -45.6(2) 19_565 .
O3 Mo1 O1' Si 128.9(3) 18 .
O3 Mo1 O1' Si 45.6(2) 4_565 .
O3 Mo1 O1' Si -128.9(3) . .
O1' Mo1 O1' Si 0.0 19_565 .
O2 Mo1 O1' Mo2 48.7(2) . 18
O3 Mo1 O1' Mo2 -176.9(3) 19_565 18
O3 Mo1 O1' Mo2 -2.5(3) 18 18
O3 Mo1 O1' Mo2 -85.8(4) 4_565 18
O3 Mo1 O1' Mo2 99.8(5) . 18
O1' Mo1 O1' Mo2 -131.3(2) 19_565 18
O2 Mo1 O1' Mo2 -48.7(2) . .
O3 Mo1 O1' Mo2 85.8(4) 19_565 .
O3 Mo1 O1' Mo2 -99.8(5) 18 .
O3 Mo1 O1' Mo2 176.9(3) 4_565 .
O3 Mo1 O1' Mo2 2.5(3) . .
O1' Mo1 O1' Mo2 131.3(2) 19_565 .
O5 Mo2 O1' Si -174.6(7) . .
O3 Mo2 O1' Si 125.9(7) . .
O7 Mo2 O1' Si 41.8(6) . .
O4 Mo2 O1' Si -130.6(7) . .
O6 Mo2 O1' Si -47.3(6) . .
O1 Mo2 O1' Si -0.7(4) . .
O5 Mo2 O1' Mo1 56.9(10) . .
O3 Mo2 O1' Mo1 -2.6(3) . .
O7 Mo2 O1' Mo1 -86.7(3) . .
O4 Mo2 O1' Mo1 100.9(5) . .
O6 Mo2 O1' Mo1 -175.8(4) . .
O1 Mo2 O1' Mo1 -129.2(5) . .
O5 Mo2 O1' Mo2 -39.2(11) . 18
O3 Mo2 O1' Mo2 -98.7(4) . 18
O7 Mo2 O1' Mo2 177.1(3) . 18
O4 Mo2 O1' Mo2 4.8(4) . 18
O6 Mo2 O1' Mo2 88.0(4) . 18
O1 Mo2 O1' Mo2 134.6(6) . 18
O5 Mo2 O3 Mo1 -155.7(7) . .
O7 Mo2 O3 Mo1 102.7(7) . .
O4 Mo2 O3 Mo1 -56.5(8) . .
O6 Mo2 O3 Mo1 23.4(17) . .
O1' Mo2 O3 Mo1 4.3(6) . .
O1 Mo2 O3 Mo1 39.9(8) . .
O2 Mo1 O3 Mo2 156.1(6) . .
O3 Mo1 O3 Mo2 -105.8(6) 19_565 .
O3 Mo1 O3 Mo2 57.7(9) 18 .
O3 Mo1 O3 Mo2 -23.9(6) 4_565 .
O1' Mo1 O3 Mo2 -41.7(7) 19_565 .
O1' Mo1 O3 Mo2 -4.4(6) . .
O5 Mo2 O4 Mo2 155.9(9) . 18
O3 Mo2 O4 Mo2 53.9(10) . 18
O7 Mo2 O4 Mo2 -29.9(18) . 18
O6 Mo2 O4 Mo2 -105.5(10) . 18
O1' Mo2 O4 Mo2 -8.3(8) . 18
O1 Mo2 O4 Mo2 -42.1(10) . 18
O5 Mo2 O6 Mo2 -155.4(11) . 20_655
O3 Mo2 O6 Mo2 25(2) . 20_655
O7 Mo2 O6 Mo2 -53.6(11) . 20_655
O4 Mo2 O6 Mo2 106.1(12) . 20_655
O1' Mo2 O6 Mo2 42.8(11) . 20_655
O1 Mo2 O6 Mo2 7.2(10) . 20_655
O5 Mo2 O7 Mo3 154.7(7) . .
O3 Mo2 O7 Mo3 -103.7(7) . .
O4 Mo2 O7 Mo3 -19.4(15) . .
O6 Mo2 O7 Mo3 55.7(8) . .
O1' Mo2 O7 Mo3 -38.9(7) . .
O1 Mo2 O7 Mo3 -5.8(6) . .
O8 Mo3 O7 Mo2 -156.5(6) . .
O7 Mo3 O7 Mo2 23.5(6) 2_665 .
O7 Mo3 O7 Mo2 -56.8(9) 20_655 .
O7 Mo3 O7 Mo2 104.0(6) 19_565 .
O1 Mo3 O7 Mo2 5.9(6) . .
O1 Mo3 O7 Mo2 39.4(7) 2_665 .
